Synthesis and Properties of Dimetallic M1[Pz]-M2[Schiff Base] Complexes
Min Zhao; Chang Zhong; Charlotte Stern; Anthony G. M. Barrett; Brian M. Hoffman; Inorganic Chemistry 43 (2004) 3377–3385; doi:10.1021/ic035402x

data_4311053
_publ_section_title
;
 Synthesis and Properties of Dimetallic M1[Pz]-M2[Schiff Base] Complexes
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3377
_journal_page_last               3385
_journal_paper_doi               10.1021/ic035402x
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'C65.5 H70 N10 Ni1.07 O2.75'
_chemical_formula_weight         1104.15
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                104.000(4)
_cell_angle_beta                 96.000(4)
_cell_angle_gamma                95.000(4)
_cell_formula_units_Z            2
_cell_length_a                   10.427(2)
_cell_length_b                   14.848(3)
_cell_length_c                   21.418(5)
_cell_measurement_reflns_used    0
_cell_measurement_temperature    153.2
_cell_measurement_theta_max      0.0
_cell_measurement_theta_min      0.0
_cell_volume                     3178.0(12)
_computing_cell_refinement       'Bruker SAINT-1000 Diffractometer Control'
_computing_data_collection       'Bruker SMART-1000 Diffractometer Control'
_computing_data_reduction        'Bruker SAINT-1000 Diffractometer Control'
_computing_publication_material  'teXsan for Windows (MSC, 1997)'
_computing_structure_refinement  'teXsan for Windows (MSC, 1997)'
_computing_structure_solution
;
SIR92 (Altomare, et. al. 1993)
;
_diffrn_ambient_temperature      153.2
_diffrn_measurement_device       'Bruker SMART-1000 CCD'
_diffrn_measurement_method       \w\
_diffrn_orient_matrix_UB_11      0.00000
_diffrn_orient_matrix_UB_12      0.00000
_diffrn_orient_matrix_UB_13      0.00000
_diffrn_orient_matrix_UB_21      0.00000
_diffrn_orient_matrix_UB_22      0.00000
_diffrn_orient_matrix_UB_23      0.00000
_diffrn_orient_matrix_UB_31      0.00000
_diffrn_orient_matrix_UB_32      0.00000
_diffrn_orient_matrix_UB_33      0.00000
_diffrn_radiation_detector       'scintillation counter'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Sealed tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.05542
_diffrn_reflns_av_sigmaI/netI    0.095
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            29187
_diffrn_reflns_reduction_process 'Lp corrections applied'
_diffrn_reflns_theta_max         28.48
_diffrn_reflns_theta_min         0.99
_diffrn_standards_decay_%        0.00
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.376
_exptl_absorpt_correction_T_max  1.000000
_exptl_absorpt_correction_T_min  0.669768
_exptl_absorpt_correction_type   'empirical SADABS'
_exptl_crystal_colour            opaque
_exptl_crystal_density_diffrn    1.154
_exptl_crystal_density_meas      ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             1169.92
_exptl_crystal_size_max          0.56
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.45
_refine_diff_density_min         -0.70
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   2.919
_refine_ls_goodness_of_fit_ref   3.900
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     669
_refine_ls_number_reflns         16753
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1820
_refine_ls_R_factor_gt           0.093
_refine_ls_shift/su_max          0.0500
_refine_ls_shift/su_mean         0.0008
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w = 1/[\s^2^(Fo)]'
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.2130
_refine_ls_wR_factor_ref         0.103
_reflns_number_gt                16753
_reflns_number_total             14681
_reflns_threshold_expression     I>3.00\s(I)
_cod_data_source_file            ic035402xsi20040325_015332.cif
_cod_data_source_block           '_s16k'
_cod_original_cell_volume        3178.1(12)
_cod_original_sg_symbol_H-M      'P -1 '
_cod_original_formula_sum        'C65.50 H70 N10 O2.75 Ni1.07 '
_cod_database_code               4311053